Abstract
The quest for designing new selfpropelled colloids is fuelled by the demand for simple experimental models to study the collective behaviour of their more complex natural counterparts. Most synthetic selfpropelled particles move by converting the input energy into translational motion. In this work we address the question if simple selfpropelled spheres can assemble into more complex structures that exhibit rotational motion, possibly coupled with translational motion as in flagella. We exploit a combination of induced dipolar interactions and a bonding step to create permanent linear bead chains, composed of selfpropelled Janus spheres, with a wellcontrolled internal structure. Next, we study how flexibility between individual swimmers in a chain can affect its swimming behaviour. Permanent rigid chains showed only active rotational or spinning motion, whereas longer semiflexible chains showed both translational and rotational motion resembling flagella likemotion, in the presence of the fuel. Moreover, we are able to reproduce our experimental results using numerical calculations with a minimal model, which includes full hydrodynamic interactions with the fluid. Our method is general and opens a new way to design novel selfpropelled colloids with complex swimming behaviours, using different complex starting building blocks in combination with the flexibility between them.
Similar content being viewed by others
Introduction
Active or selfpropelled colloidalparticle systems are currently a subject of great interest in soft condensed matter science, owing to their ability to mimic the collective behaviour of complex living systems, but also to serve as model systems to study intrinsically outofequilibrium systems^{1,2,3,4,5,6}. Selfpropelled particles can exhibit rich collective behaviour, such as clustering, segregation, and anomalous density fluctuations, by consuming internal energy or extracting energy from their local environment in order to generate their own motion^{1,2,3,4,5,7}. In recent years, several experimental selfpropelled particle systems have been developed, namely Janus spherical particles^{2,8,9,10,11}, Janus rods^{12}, bimetallic rods^{13}, granular rods^{14}, gearshaped^{15,16}, heterodimers^{17}, and Lshaped particles^{18}, based on different selfpropulsion mechanisms. However, most of the experimental studies have been reported on Janus spherical^{19} and rodlike particle systems^{12}. Moreover, the majority of selfpropelled particles move actively by converting the input energy directly into translational motion on a single particle level. As a result, the selfpropelled particles exhibit ballistic behaviour at time scales much smaller than the rotational diffusion time and diffusive behaviour at longer time scales, with an effective diffusion coefficient that is many times larger than the equilibrium diffusion coefficient. In this work we ask ourselves whether, and if so how, selfpropelled Janus spheres can assemble into bead chains that exhibit rotational motion, possibly coupled with translational motion. Some biological systems display active rotational motion, e.g., certain bacteria confined to two dimensions^{20}, and dancing algae^{21}. To the best of our knowledge, only a few synthetic systems show active rotation, e.g., a granular gearshaped particle in an active bacterial bath^{15,16}, multilayered bimetallic rods^{22,23}, Lshaped particles^{24}, and random clusters of active Janus particles^{25,26}. However, the swimming behaviour of these systems cannot be tuned by controlling the internal structure. Here, we develop a new type of internally driven colloidalparticle system, namely selfpropelled colloidal bead chains with tunable stiffness. This system is suitable to study dynamics on a single particle level in concentrated systems, and exploits directed selfassembly of simple selfpropelled building blocks. Moreover, we show that introducing (semi)flexibility between the beads in a chain is sufficient to break the timereversibility constraint to realize flagellumlike or helicallike motion that is powered by the fuel. To the best of our knowledge, flagellumlike motion has not been reported before in internally powered (selfpropelled) colloidal swimmers. Only externally powered propellers such as helixshaped^{27,28,29,30} particles using rotating magnetic fields, and DNAlinked assemblies of magnetic particles tethered to a red blood cell^{31} in biaxial magnetic fields have shown this motion. However, these systems are not suitable for collective behaviour studies because the longranged magnetic interactions between individual units are difficult to minimize. Additionally, they do not satisfy the forcefree and torquefree condition^{28} which is an essential condition for studying internally powered colloidal systems. Moreover, these systems are difficult to fabricate.
Several simulations and theoretical studies have predicted that particle shape and swimming direction can affect the macroscopic behaviour of selfpropelled particle systems^{1,2,6,32}, but the experimental realization of shapeanisotropic particles in combination with varying propulsion directions scarcely exists. Several synthesis routes have been reported for synthesizing ‘passive’ colloidal molecules, complexshaped particles^{33,34,35,36,37,38}, chains of particles using different starting building blocks, e.g., isotropic spherical particles using various linking mechanisms^{34,39,40,41,42}, Janus particles^{43}, and flattened particles^{44}. However, making these model systems with selfpropelling capabilities remains a challenge. Here, we take an inspiration from the design principles of synthesizing passive colloidal molecules, where the colloidal spherical particles are treated as atoms and the interactions between them are tuned such that they selfassemble into welldefined complex clusters^{33,34,36}. We show that selfassembly of the Janus particles into polymerlike chains with tunable stiffness provides a powerful route towards the fabrication of complex selfpropelled particle systems.
Fabrication of permanent bead chains
We first present our method to create catalytically powered colloidal rotators or active rigid linear bead chains by connecting the individual selfpropelled spherical swimmers in such a way that neighbouring swimmers in the chain are always propelling in opposite directions. Our fabrication method consisted of two steps (Fig. 1a): (i) aligning Janus particles into linear chains using a high frequency external AC electric field^{45}, and (ii) making these structures permanent using a combination of van der Waals attractions and linkers (i.e., interdiffusion of polymer chains that are made of particles, and polyelectrolytes) to ensure that the chains remained intact as a chain even after removing the field. Suspensions consisting of 0.02 vol% halfside Pt coated polystyrene (PS) particles in deionized water were introduced to a rectangular electric cell (0.1 × 1.0 mm^{2}). Upon application of a high frequency external AC electric field (E _{ rms } = 0.01 Vμm^{−1}, f = 800 kHz where E _{ rms } is the rootmeansquare electricfield strength and f is the frequency), the particles assembled into staggered or zigzag linear chains in the direction of the applied field (Fig. S1b). The difference in the polarizability of both sides (halfdielectric and halfmetallic) of the Janus particles caused the particles to align into staggered chains as shown in Fig. S1b. At low particle concentrations and at low field strengths, the stable structure is a string fluid phase that consists of staggered chains of particles in the field direction and a liquidlike order in the
perpendicular to the field direction (Fig. S1b)^{45}. However, these linear structures rely on the presence of external electric fields, i.e., the chains lost their identity (Fig. S1c) when the field was switched off ^{37,45}. To circumvent this, we used a combination of a strong electric field and a heating step. At high field strengths (E _{ rms } = 0.04–0.05 Vμm^{−1}, f = 800 kHz), the induced dipolar attractions between the particles are strong enough to push the particles together into distances where the van der Waals attractions take over and bind the particles irreversibly. In particular, the van der Waals attractions between metallic halves of the particles are strong in comparison to those between the polymeric halves of the particles^{46}. Due to some irregularities in the Pt coating a small fraction of the polymeric side of a particle can also touch the polymeric side of neighbouring particles. These polymerpolymer connections are the key to making permanent bonds between neighbouring Janus spheres through a heating step that was developed in an earlier study by Vutukuri et al.^{34,39}. In the heating step, the sample cell was heated to 60–65 °C, which is well below the glass transition temperature^{47} (T _{ g } ≈ 107 °C) of polystyrene as shown in Fig. S2, for about 2–3 minutes using a hotair stream that was much wider than the sample cell^{34,39}. After 2–3 minutes, the field was slowly switched off and we found that the particles were permanently attached to each other in a staggered fashion and acted as a single rigid body. Fig. S3 shows the length distribution of the resulting permanent bead chains. It is important to mention here that the length of the permanent chains can be controlled by varying the distance between the two electrodes as has been developed in our previous study by Vutukuri et al.^{34}. This procedure could thus significantly increase the monodispersity in length, if necessary, but was not used in the present study.
Results and Discussion
Dynamics of selfpropelled rotators or active rigid bead chains
After creating the permanent structures, we studied their dynamic behaviour in the presence of H_{2}O_{2}. We note that it has been reported that in the case of individual half Ptcoated Janus spheres, the platinumcatalyzed decomposition reaction of H_{2}O_{2} generates a concentration gradient of ions across the surface of the particles, inducing selfpropulsion in the direction of the noncoated surface^{8,9,10,48}. Although the underlying mechanism responsible for the propulsion is still under debate^{49}, the dominant propulsion mechanism is probably a combination of diffusiophoresis and selfelectrophoresis^{8,9,10,48}. When we transferred the permanent staggered chains into a 1.0 vol% H_{2}O_{2} solution, the bead chains showed autonomous sustained rotating behaviour on the surface of the bottom wall (Fig. 1b). The rotating movement can be attributed to the fact that the propulsion force on each Janus particle is acting in opposite directions in alternative fashion along the length of the chain (see the inset of Fig. 1b), resulting in a constant torque acting on the chain, which induces a rotational motion of the chain. The timelapsed bright field images show the rotational motion of a 6bead chain in 1.0 vol% of H_{2}O_{2} solution as shown in Fig. 1b (see supplementary Movie S1). The inset of Fig. 2b shows the typical trajectory of the centreofmass of the bead chain. In order to characterize the trajectories, we first extracted the centroids of each bead (Janus spheres) in a chain using a particletracking algorithm^{50}, and then calculated the orientation angle based on the coordinates of the first and the last bead as a function of time (see Materials and Methods section). From this, we calculated the meansquared angular displacement (MSAD), and the translational meansquared displacement (MSD) of the centre of mass of the chain as shown in Fig. 2. Due to the persistent angular propulsion, the bead chains are actively rotating, as shown by the cumulative rotational angle θ(t) continuously increasing with time (inset of the Fig. 2a). We obtained the average angular velocity (ω) and the passive (equilibrium) rotational diffusion coefficient (D_{r,eq}) of the rotator by fitting the MSAD curves with the equation \(\langle {\theta }^{2}\rangle =\langle {[\theta (t)\theta (0)]}^{2}\rangle ={\omega }^{2}{t}^{2}+2{D}_{r}t\) (see more details in Materials and Methods section). The rotator or active bead chain was propelling with an angular velocity ω = 0.48 ± 0.03 rad/s. The obtained equilibrium rotational constant,
D_{r,eq} = 0. 005 ± 0.004 rad^{2}/s, is consistent with the theoretical value^{51} as well as with our numerical calculations (see the beadshell minimal model in Materials and Methods section). Note that at the same fuel concentration (1.0 vol% of H_{2}O_{2} solution), singlets propelled with a velocity of 1.58 μm/s (see Fig. S4). In contrast to single selfpropelled spheres, our rotators show distinctive MSAD and MSDs. The main distinctive feature of the MSD is an oscillatory behaviour indicating that the rotator performs a spirallike “spira mirabilis” motion due to thermal fluctuations. As shown in Fig. 2b, the experimental MSD is in a good quantitative agreement with the theoretical predictions as have been reported for a thin rod with not only a selfpropulsion force, but also a selfpropulsion torque, i.e., a circular swimmer^{52}. We note that the angular velocity obtained from the MSAD fitting (ω = 0.48 ± 0.03 rad/s) is in quantitative agreement with the value obtained from the MSD fitting (ω = 0.42 ± 0.09 rad/s). Next, we quantified the dynamics of bead chains in terms of angular velocity for different chain length and at different fuel concentrations. For each fuel concentration, we analysed 6 trajectories for each chain length in two separately prepared samples. In Fig. 3, we plot the average angular velocity as a function of chain length, for two different fuel concentrations. It is apparent from Fig. 3 that the chains with an even number of beads exhibit rotations that are much more pronounced than those of chains with an odd number of beads. This can be understood from the forces on the beads: in a perfectly symmetric chain where the propulsion forces are antiparallel, a chain with an even number of beads will experience a net torque, but no net force. In contrast, a chain with an odd number of particles will experience no net torque but will experience a net force. In practice, small asymmetries result in both forces and torques on both types of chains, but the preference of oddnumbered chains for translation and evennumbered chains for rotation is preserved. Both clockwise (CW) and counterclockwise (CCW) rotations are observed for different chain lengths. For longer bead chains (>3σ, where σ is the particle diameter) the gravitational height of the passive bead chains is l _{ g } > 1.0 μm, which is comparable to the particle diameter. As a result, they are confined to a plane where they, once started rotating in a particular direction, tend to continue in that direction. We did not observe any switching between the directions from the CCW to the CW directions and vice versa. On the other hand, for dimer and trimer chains we did observe switching between the rotation directions. This can be attributed to the fact that the gravitational height for shorter bead chains is less than one particle diameter. For instance, the gravitational height of a dimer bead chain is ~0.3 σ. As a consequence, shorter chains do not only show small fluctuations out of the 2D plane, but show also full rotations in 3D, thereby switching between CCW and CW rotation directions. For an even number of beads in a chain, the angular velocity decreases with increasing length at constant fuel concentration, as shown in Fig. 3. In order to capture the flow fields generated by the rotators in the fluid, we added uncoated PS spheres of diameter 2.1 μm as tracer particles in the sample cell. We subsequently followed the dynamics of the tracer particles as a function of time by means of a bright field microscope. The trajectories of the tracer particles reveal that the tracer particles in close proximity of the 4bead rotator show net motion (Fig. 4), while the particles far from the rotator show Brownian motion and the effect of the rotator is negligible in this case. Based on our experimental observations we believe that there is no bulk convective flow present in the system.
Selfpropelled or active semiflexible bead chains
Next, we study how flexibility between the beads in a chain affects the swimming behaviour in the presence of a fuel. Here we used sterically stabilized PS (polystyrene) Janus particles with a high molecular weight polyvinylpyrrolidone (PVP, M_{w} = 360 kg mol^{−1}) as starting building blocks and repeated the same protocol as was mentioned for the fabrication of active rigid chains. The particles that were sterically stabilized with a higher molecular weight PVP form chains with a semiflexible character^{34} as the stabilizing polymers (PVP) that were chemically connected and/or entangled with the PS polymer chains, acted as linkers between the beads. Using Fourier mode analysis, we quantified the flexibility of the resulting chains by estimating the persistence length l _{ p }, yielding l _{ p } ≈ 20σ, where σ is the diameter of a bead^{34}. When we introduced flexibility between the beads in a chain, the resulting chains showed a completely different swimming behavior consisting of a coupled translational and rotational motion, which strongly resembles flagellumlike motion or helical motion (see supplementary Movie S2). Here, our intention is to refer to the observed swimming behavior as a flagellalike motion, which means that the chain is undergoing an intricate coupling between rotational and translational motion. We note that the rigid bead chains showed only active rotational motion. The timelapsed bright field images show the sequential shape and orientation changes of an active semiflexible chain, indicated by the change in intensity of beads in the chain as shown in the XY projection in Fig. 5a. We further confirmed this by measuring the intensity profile of the uncoated side of the third bead in the chain, which shows oscillatory behavior with time (Fig. 5c). We note that the bright parts of the beads in the chain indicate the uncoated side of the bead in the focal plane, while the dark ones indicate beads that are either above or below the focal plane. Next, we analyzed the motion of the chain in the orthogonal XZ view, which reveals the spiral motion of the chain (Fig. 5b). Figure 5d demonstrates a typical trajectory of the center of mass of the active semiflexible bead chain during a time interval of 20 seconds. The resulting conformations and propulsion motion is a consequence of a coupling between the propulsion forces, chain flexibility and viscous drag from the solvent that generates controlled deformations. As our chains are semiflexible in nature (persistence length, l _{ p } ≈ 20 σ; contour length, l _{ c } ≈ 6 σ), we expect that there is always some correlation between the neighboring particles, since a combination of flexibility of the chain and hydrodynamic forces may generate an asymmetry in the selfpropulsion direction of the beads. As a result, the rotation cycle is nonreciprocal, leading to (see supplementary Movie S2) a net translational displacement of the chain^{28,53}. Next, we examined the flows generated in the fluid by a selfpropelled 6bead chain, by means of a 1.0 μm tracer particles and a 5.0 μm elongated glass piece (a contamination in the sample cell). The typical trajectories of tracers over 20 sec are shown in Fig. 5e. One clearly deduces from the paths of the tracer particles that there is no bulk convective flow present in the system.
In the presence of 1.0 vol% H_{2}O_{2}, the chain showed both rotational and translational motion. The active rotational velocity around the axis of the active 6bead semiflexible chain (Fig. 5) is 3.5 rad/sec and the chain is propelling along the long axis with a velocity of 0.9 μm/s. The chain of 8 beads propelled with a translational velocity of 0.62 μm/s and the rotational velocity around the axis is 3.8 rad/sec in 1.0 vol% H_{2}O_{2} solution. Due to the large persistence length (l _{ p } ≈ 20 σ) of the semiflexible chains, the shorter chains (≤4σ) behaved like rigid chains and showed rotator behaviour.
In addition, we will demonstrate now that our method can also be used to make more complex selfpropelled chains composed of both semiflexible and rigid parts as shown in Fig. 6. These complex chains were fabricated by mixing rigid and semiflexible chains together and repeating the same protocol as was used in making the constituent bead chains. In the presence of fuel (1.0 vol% H_{2}O_{2}), the propelling behaviour (see supplementary Movie S3) of a halfrigid and halfsemiflexible 8bead chain resembles the swimming behaviour of microorganisms with a flexible tail and a rigid head, such as e.g., E. coli. The rotational velocity of the long axis of the halfrigid and halfsemiflexible 8bead chain is 1.9 rad/sec and the propelling velocity is 1.2 μm/s. We believe that our method opens up new possibilities to realize more complex swimmers, for instance, attaching a semiflexible chain to a ‘passive’ single big sphere or a cargo.
Beadshell minimal model and equations of motion
In order to better understand the experimentally observed propulsion behavior of bead chains, we complemented our study with a minimal model that includes full hydrodynamic interactions with the fluid (see more details in Materials and Methods section). Instead of modeling the catalytically powered selfpropulsion in terms of a slip velocity on the surface of the Janus particles, we model the propulsion mechanism by an effective propulsion force of a fixed magnitude that acts on each of the Janus spheres. For a rigid chain of spheres, these propulsion forces sum up to a force and torque acting on this rigid configuration. If the 6 × 6 hydrodynamic resistance tensor of this rigid body is known, the equations of motion of this object can be solved after imposing the effective force and torque. Alternatively, if the motion of the body is known, these equations of motions may be inverted to calculate the effective force and torque. We apply this to the rigid rotating chains, for which the observed angular velocity is used to calculate, given the ‘zigzag’ arrangement of the propulsion forces, the magnitude of the effective propulsion force (more details in Materials and Methods section). To check the validity of this procedure, we feed the obtained effective force magnitude back into the equation of motion, from which we calculate the angular velocity for rigid bead chains of different lengths. We found our calculations to be consistent with the experimentally measured angular velocities (Fig. 3) in all three cases of bead chains with an even number of beads, as shown in Fig. 7.
Selfpropelled semiflexible bead chains
As shown experimentally, the active rigid bead chains did not exhibit any translational motion (Figs 1b and 2), whereas the semiflexible chains showed a net translational motion (Fig. 5). Due to the overdamped nature of the dynamics at low Reynolds numbers, we expect that the internal motions within a semiflexible bead chain will quickly decay towards an equilibrium configuration, rather than showing oscillatory motion as in the case of a driven oscillator with inertia. Below we show that a small anisotropy in both the shape and the force distribution of the bead chain, induced by the semiflexibility, can lead to a translational motion of the bead chain, even when the net effective propulsion force on the chain remains zero. To this end, we analyzed small anisotropies in the shape by considering bead chains with the centers of the Janus spheres positioned in a Cshape and on a helical centerline, as parameterized by a helical radius r and helical pitch p (see more details in Materials and Methods section). In addition, we studied anisotropic arrangements of these propulsion forces that deviate from the ‘zigzag’ arrangement.
We summarized our numerical predictions in terms of ‘swimming’ behavior for the active helical bead chains with varying shape and propulsion force distributions in the Figure TI. We clearly found that anisotropy in both shape and force distribution is required to induce translational motion.
Hence, shape anisotropy in the form of a Cshaped or (moderately) helically shaped bead chain, combined with a heterogeneous distribution of propulsion forces, leads to a ‘swimming’ motion that qualitatively reproduces the experimentally observed propulsion behavior (Fig. 5). This can also be clearly seen in animation 6 found in the Supplementary information. We now take a close look at the influence of the force distribution on the swimming behavior. In Fig. 8, we compare the inplane (projected) velocity v _{2D} and angular velocity around the long axis of the bead chain, ω _{}, for a set of 100 randomly chosen configurations of propulsion forces for a fixed helically shaped bead chain, to the (angular) velocity for a range of different helical bead chains and the experimentally observed values. Here, we considered configurations with 6 randomly chosen orientations (blue), which are (almost) never forcefree. In addition, we considered zigzag configurations with a single randomly chosen orientation (purple), as well as configurations with three randomly chosen directions of propulsion forces, augmented with the three opposite vectors. For the latter two categories, the total effective propulsion force vanishes. From Fig. 8, we observed that these random configurations do not produce translational motion that qualitatively agrees with the observed experimental motion and therefore we conclude that the arrangement of the effective propulsion forces requires a certain correlation of the directions of the forces on the beads. Since the experimental system is semiflexible in nature (persistence length, l _{ p } ≈ 20σ; contour length, l _{ c } ≈ 6σ) and initially made from a linear zigzag beadchain, there are always correlations between the force directions of neighboring beads in the chain.
Conclusions
In conclusion, we have developed an effective, yet simple method for the fabrication of internally powered colloidal bead chains with tunable stiffness. Our active bead chains are the first experimental realization of a new type of selfpropelled particles that spontaneously rotate or spin when the spherical swimmers are rigidly connected, while they show flagellumlike propulsion when the connections between the spherical swimmers are semiflexible. In the presence of the fuel, active rigid bead chains experience equal and opposite propulsion forces along the length of the chain that induce active rotational motion. Due to the hydrodynamic forces and the flexibility of the chain, long (≥6σ) selfpropelled semiflexible chains are subject to asymmetry in the selfpropulsion direction of the beads in a chain, leading to flagellumlike motion. We corroborated our experimental results by means of numerical calculations with a minimal theoretical model, based on a description via effective propulsion forces. We were able to reproduce qualitatively and to some extent quantitatively, the ‘swimming’ behavior of the semiflexible bead chains. Also, the spiraling motion calculated from this model agrees well with the experimentally observed motion of the bead chains. With our numerical calculations we found that the propulsion forces along the chain require some correlations between the directions of the forces on the beads to induce translational motion for active semiflexible chains. These correlations may arise from the semiflexible nature of the chains that initially had a welldefined linear zigzag structure. Our findings demonstrate how microscopic dynamics (i.e., flexibility between the beads) can affect the dynamical behavior of selfpropelled bead chains. In future studies, the length of the chains can be controlled using previously reported methods by Vutukuri et al.^{34}. Potentially, our method paves a way to study collective behavior of selfpropelled or internally driven chains with tunable stiffness, and can likely be extended to lightactivated propelling particles^{7} (e.g., halftitania coated particles) where the rotational speed of rigid chains and the swimming speed of semiflexible bead chains can be controlled with light intensity. Additionally, we can easily extend the procedure to magnetodielectric particles such as magnetic nanoparticles embedded in micronsized polymeric particles, so that we can control the directionality of the motion of active bead chains by either external magnetic or electric fields. This work will facilitate future designs of new complex selfpropelled swimmers, for instance, attaching a ‘passive’ single big sphere or a cargo with an active semiflexible bead chain.
Materials and Methods
Particle synthesis
We synthesized^{54} electrostatically stabilized and negatively charged polystyrene (PS) particles of 1.35 μm with a size polydispersity of 4%, and sterically stabilized (polyvinylpyrrolidone, PVP, M_{w} = 40 kg/mol) with a size polydispersity of 3%. These two types of particles were used in the fabrication of rigid bead chains. Whereas a longer molecular weight PVP (M_{w} = 360 kg/mol) PS particles were used in the fabrication of semiflexible bead chains. Sterically stabilized PS particles were synthesized using the method of Song et al.^{55}. The size of the sterically stabilized PS particles was 1.40 μm with a size polydispersity of 5%. The particle size and polydispersity were determined using static light scattering, and scanning electron microscopy. We note that based on our camera frame rate, we deemed it easier to follow the dynamics of tracer particles in the case of rigid bead chains when we used bigger particles (2.1μm), because the chains are rotating faster. On the other hand, smaller particles (1.0 μm) are sufficient to capture the dynamics of tracer particles in the case of semiflexible case.
Janus particles preparation
We first prepared a monolayer of spherical particles by slowly drying particles from a dilute suspension (0.05 wt%) on a clean microscope glass slides. A 15 nm thick layer of platinum (Pt) was then vertically deposited using a sputter coater (Cressington 208HR). Prior to particle detachment, slides were thoroughly washed with DI water, and subsequently particles were detached by sonicating the slides in DI water for 10 mins. Next, particles were washed a couple of times with DI water and then the suspension with the desired concentration was transferred to the electric cell.
Electricfield setup
The electric cell consisted of a 0.1 mm × 1.0 mm cross section capillary with two 50 µm thickness nickelalloy wires (Goodfellow) threaded along the side walls^{56,57}. We used a function generator (Agilent, Model 3312 OA) and a wide band voltage amplifier (KrohnHite, Model 7602M) to generate the electric fields. We used a high frequency AC fields to minimize the polarization effects of the electric double layer around the particle. The field strength and the frequency were measured with an oscilloscope (Tektronix, Model TDS3052). We used a homemade DC filter to remove the DC component in the signal.
Fixation of bead chains
After filling the cell with the Janus colloidal particles suspension, we sealed both ends of the capillary with UVcuring optical adhesive (Norland No. 68) and cured the glue with UV light (λ = 350 nm, UVGL58 UV lamp). The dispersion was then exposed to an AC field (E _{ rms } = 0.04–0.05 Vμm^{−1}, f = 800 kHz), and the ramping time was about 2 mins. After 2–3 mins, all the particles were assembled into zigzag chains of one particle wide in the field direction. The dispersion was subsequently heated to 60–65 °C, which is well below the glass transition temperature (T _{ g } ≈ 107 °C) of polystyrene^{47}, for about 2–3 minutes using a hotair stream that was much wider than the sample cell^{34,39,58}. We further kept the field on for 2–3 mins while the sample was cooled down to room temperature. After the fixation step, we carefully opened both ends of the electric cell and the bead chains were subsequently transferred to a small eppendrof tube (0.5 ml) for further dilution. The dynamics of the chains were studied in LabTek chambered coverglass (Thermo Fisher Scientific).
Internal structure of staggered or zigzag chains
Our method yielded regular and staggered (zigzag) linear chains independent of whether it is used in the fabrication of rigid or semiflexible chains. We note that in our fabrication method, we exploited the difference in the polarizability of both sides (halfdielectric and halfmetallic) of the Janus particles in external AC electric fields, causing a zigzag chain configuration, as is shown in the Fig. S1. In the case of semiflexible (persistence length, l _{ p } ≈ 20 σ; contour length, l _{ c } ≈ 6 σ), we expect that there remains always some correlation between the neighboring particles, stemming from the zigzagged pattern at synthesis, while a combination of flexibility of the chain and hydrodynamic propulsion may generate an asymmetry in the selfpropulsion direction of the beads.
Particle tracking
We recorded the particle dynamics using an Olympus IX81 confocal microscope, equipped with an Andor iXon3 camera, Andor 400series solidstate lasers, a Yokogawa CSUX1 spinning disk. Brightfield optical micrographs and videos were recorded using a Nikon microscope equipped with a CCD camera (Olympus CKX41). We processed recorded images and extracted the centroids of each particle in a chain using the particle tracking programs of Rogers et al.^{50}. We then calculated the orientation of the chain from the pixel coordinates of the first bead and the last bead in the chain. To uniquely identify the both ends of the chains, it is required that the rotation angle of the chain between successive frames is less than π/2.
Mean squared displacement of rigid chains
The MSAD and MSDs can be determined by solving the equations of motion for a circular swimmer^{52}. The overdamped equations can be written in 2D as
where ω is the rotational velocity, x and y are the center of mass coordinates, \(\nu \) is the propulsion velocity, and θ is the orientation of the bead chain. The Brownian noise terms, \(\xi \), \(\zeta \), are Gaussian random variables with zero mean whose magnitudes are taken from theoretical Brownian diffusivities. By solving the Eqs 1–3 we obtained
where D _{ r } is the rotational diffusion coefficient, \({D}_{\parallel }\), \({D}_{\perp },\) are translational diffusion coefficients along the major and minor axis, and \(v\) is the propulsion velocity.
Resistance tensor, beadshell model and equations of motion
Often, the catalytically powered selfpropulsion of (half)platinum coated particles, such as the bead chains considered this work, is modelled by a slipvelocity on the active part of the particle surface. Moreover, since there are no external forces acting on the bead chains, the total hydrodynamic force and torque on the chain both vanish, such that the flow field around the bead chain is, to leading order, at most of dipolar character. However, as was proven by Ten Hagen et al.^{59}, the motion of a selfpropelled particle is equivalent to that of a passive particle (of identical shape), which is driven by an effective external force F ^{eff} and torque T ^{eff}. As described in ref.^{59}, if both the distribution of slipvelocity on the active particle surface, and flow field solutions around the driven passive particle for arbitrary external force and torque are known, the motion of the active particle may be solved by taking suitable choices of the driving forces in the conjugate passive particle system. Subsequently, the effective force F ^{eff} and torque T ^{eff} are calculated from the passive case by imposing the velocity and angular obtained in the previous step. Due to the linearity of lowReynolds number hydrodynamics, the force and torque relate to the particle velocity U and angular velocity ω in a linear fashion:
where the 6vector \({\mathscr{F}}=({{\boldsymbol{F}}}^{{\boldsymbol{e}}{\boldsymbol{f}}{\boldsymbol{f}}},{{\boldsymbol{T}}}^{{\boldsymbol{e}}{\boldsymbol{f}}{\boldsymbol{f}}})\) denotes the (effective) force and torque on the particle, the 6vector \({\mathscr{V}}=({\boldsymbol{U}},{\boldsymbol{\omega }})\) denotes the (angular) velocity with respect to a chosen reference frame and the 6 × 6 tensor \( {\mathcal R} \) denotes the hydrodynamic resistance tensor, which depends itself on the shape of the selfpropelled particle under consideration. The linearity of this dependence is due to the linearity of the Stokes equation that governs the hydrodynamics at low Reynolds numbers.
Here, rather than calculating the effective force and torque from the slipvelocity on the active bead chains, and flow field solutions of the passive problem, we adopt the opposite strategy by directly determining the effective force and torque from bead chain systems for which both the motion and the geometry are accurately known (from the experiment). To this end, we numerically (using a beadshell model, see p. 21) determine the tensor \( {\mathcal R} \) for the rigid bead chains, for which the (angular) velocity is measured in the experiment: U = 0, while \({\boldsymbol{\omega }}=\omega \hat{{\boldsymbol{z}}}\), which leads to \({{\boldsymbol{F}}}^{eff}=0\) and \({{\boldsymbol{T}}}^{eff}={T}^{eff}\hat{{\boldsymbol{z}}}\), where \({T}^{eff}\) is solved from the equation of motion \({\mathscr{F}}=\eta \,{\mathscr{R}}\,{\mathscr{V}},\) after we determined the resistance tensor \( {\mathcal R} \).
To proceed, we decompose the effective force and torque into effective forces acting on each of the individual Janus sphere that constitute the chain, as
where we assume that the force magnitude F _{ i } is equal for all i, while the direction is determined by the orientation of the catalytic hemispheres: pointing along the axis that connects the ‘south’ pole on the passive hemisphere to the ‘north pole’ of the active hemisphere, as is shown in e.g. Fig. 9 of the main text. This assumption is equivalent to assuming that the (chemical) interaction between catalytic surfaces is small, such that all F _{ i } are of equal magnitude, and that the symmetry of the active hemisphere is preserved such that (effective) contributions of individual torques on each Janus sphere may be neglected, as would be the case of a single Janus sphere. Since an alternating (‘zigzag’) orientation of the active hemispheres is clearly observed in the experiment, the magnitude F _{ i } is the only unknown and may be solved by plugging Eq. (7) into Eq. (6) for the rigid rotating chains, as described in the next section.
In this work, we calculate the rigid body resistance tensor of (active) bead chains using a beadshell model^{60,61}, in which the surface of a rigid body is homogeneously covered by a large number (M) of small spheres of radius a. When this cluster of M spheres is given a nonzero common velocity, a disturbance flow field is created, which in turn causes hydrodynamic interactions between the small spheres that are given by the RotnePrager mobility tensor^{62,63}. The forces on the individual spheres can then be calculated by a 3 M × 3 M matrix inversion, from which the total force and torque on the rigid body follow as the sum of the individual forces and torques around a chosen reference point. Subsequently, these results are extrapolated to \(M\to \infty \), while keeping Ma ^{2} finite, where typically \(M\) = 1000–3000 spheres are used in this procedure. In this large\(M\) limit, we retrieve the boundary integral formulation of the Stokes equation, guaranteeing accurate results for the resistance tensor \( {\mathcal R} \).
Selfpropelled rigid bead chains
We first validate our model for the active rigid bead chains by comparing the rotational diffusion coefficient for the 6bead chain as obtained from the beadshell model calculations to the experimental data. Assuming that the direction perpendicular to the plane of view of the microscope is the zaxis, the relevant rotational resistance coefficient is R _{66}, from which the rotational diffusion coefficient is expressed by the StokesEinstein relation as D _{ r } = k _{ B } T/(η R _{66}). Here, using the viscosity of water and the experimental size of the Janus spheres, we find D _{ r } = 0.0096 rad^{2}/s, which is consistent with the experimentally measured value. We included the experimental results of rotational speed of the rigid chains in the presence of the fuel and the rotational diffusivity of chains in water, and the rotational and the translational speed of semiflexible chains in the fuel in supplementary information (see Table SII).
For completeness, we give the complete resistance tensor in the below paragraph. Next, we use the measurements of the rotational velocity of the rigid bead chains to estimate the value of the effective propulsion force acting on each individual Janus sphere. Note that in each case, we try to stay as closely as possible to the observed ‘zigzag’ shape, as shown in Fig. S5, where we estimate from experimental snapshots that the angle between the vectors connecting the centers of adjacent Janus spheres is 0.15π on average. Also, the distribution of the propulsion forces is arranged in an alternating zigzag fashion.
The validity of our model and consistency of our assumptions, Eq. (7), is verified from Fig. 7 above, where we compare the experimentally observed angular velocity ω with the angular velocity that we calculate from Eq. (6) for chains of different length, where the values of F _{ i } is averaged over the data of the rigid bead chains.
The complete 6 × 6 resistance tensor of a rigid linear ‘zigzag’ bead chain of 6 beads, aligned along the xaxis, is found to be:
Selfpropelled semiflexible bead chains
With the magnitude F _{ i } determined from the rigid chains and the consistency of our assumptions checked, we apply this model to the motion of the semiflexible bead chains. As mentioned above, we model the semiflexible bead chains by introducing shape anisotropy to the rigid bead chains, such that the centers of the beads lie on a helix with radius r and pitch p. We note that the aligned chain (p → ∞) and the cshaped chain (p = 0) are special cases of this parameterization.
Moreover, we consider a propulsion force distribution along the bead chain that is arranged in such a way that the chain will start rotating around the axis that connects the two ends, when the chain does not coincide completely with this axis. The propulsion forces are all perpendicular to the axis that connects the end points of the bead chain, and differ by a rotation around this axis. Below, we denote the angular velocity around this axis by ω _{  }, while we represent the projected (2dimensional) velocity in the xyplane by v _{2D}. Note that, as in the case of the rotating rigid bead chains, the net force on the chain vanishes. Therefore, any translational motion is entirely caused by a (shapedependent) translationrotation coupling in the resistance tensor described above, and is in fact independent of our effective description using propulsion forces (that we have obtained from the rigid case).
We make a comparison between the theoretically calculated velocities associated with these bead chains and the velocity measured in the experiment, which is 0.9 µm/s = 0.64 σ/s. In Fig. S6, we plot the velocity of helical bead chains as a function of the helical radius r/σ and pitch α as obtained theoretically using our beadshell model. We observe that over a large range of shapes, the velocity is around 0.2 σ/s. We also investigate the rotational velocity ω _{  } for the same range of shapes, as shown in Fig. S7. Here, we observe a wide range of shapes that show an angular velocity ω _{  } of 3.0 s^{−1}, which compares well to the value of 3.5 s^{−1} in the experiments.
Finally, we studied the ratio between rotation and translation velocity, which as described above, is purely an effect of the shape of the bead chain and is independent of the magnitude of the effective propulsion force. In Fig. 10 we show this ratio as a function of helical shape, and observe that this ratio is around 0.08 σ for a range of helical shapes, whereas the experimentally measured ratio is 0.18 σ. We conclude that our minimal model is able to predict this ratio up to a factor of two, which is striking given the simplicity of the model. Also, the spiraling motion observed from the animations coincides well with the experimentally observed motion. A better understanding of experimental uncertainties or a more detailed hydrodynamic model may improve these predictions.
References
Elgeti, J., Winkler, R. G. & Gompper, G. Physics of microswimmerssingle particle motion and collective behavior: a review. Rep. Prog. Phys. 78, 056601 (2015).
Bialké, J., Speck, T. & Löwen, H. Active colloidal suspensions: Clustering and phase behavior. J. NonCrystalline Solids 407, 367–375 (2015).
Wang, J. & Gao, W. Nano/Microscale motors: biomedical opportunities and challenges. Acs Nano 6, 5745–5751 (2012).
Sengupta, S., Ibele, M. E. & Sen, A. Fantastic Voyage: Designing SelfPowered Nanorobots. Angew. Chem. Int. Edn. 51, 8434–8445 (2012).
Sanchez, S., Soler, L. & Katuri, J. Chemically Powered Micro and Nanomotors. Angew. Chem. Int. Edit. 54, 1414–1444 (2015).
Bechinger, C. et al. Active particles in complex and crowded environments. Rev. Modern Phys. 88, 045006 (2016).
Palacci, J. et al. Lightactivated selfpropelled colloids. Philos Trans A Math Phys Eng Sci 372, 0372 (2014).
Ginot, F. et al. Nonequilibrium equation of state in suspensions of active colloids. Phys. Rev. X 5, 011004 (2015).
Theurkauff, I., CottinBizonne, C., Palacci, J., Ybert, C. & Bocquet, L. Dynamic Clustering in Active Colloidal Suspensions with Chemical Signaling. Phys. Rev. Lett. 108, 268303 (2012).
Howse, J. R. et al. Selfmotile colloidal particles: From directed propulsion to random walk. Phys. Rev. Lett. 99, 048102 (2007).
Yan, J. et al. Reconfiguring active particles by electrostatic imbalance. Nat. Mater. 15, 1095–1097 (2016).
Vutukuri, H. R. et al. Dynamic selforganization of sidepropelling colloidal rods: experiments and simulations. Soft Matter 12, 9657–9665 (2016).
Wang, W., Duan, W., Sen, A. & Mallouk, T. E. Catalytically powered dynamic assembly of rodshaped nanomotors and passive tracer particles. Proc. Natl. Acad. Sci. USA 110, 17744–17749 (2013).
Narayan, V., Ramaswamy, S. & Menon, N. Longlived giant number fluctuations in a swarming granular nematic. Science 317, 105–108 (2007).
Sokolov, A., Apodaca, M. M., Grzybowski, B. A. & Aranson, I. S. Swimming bacteria power microscopic gears. Proc. Natl. Acad. Sci. USA 107, 969–974 (2010).
Di Leonardo, R. et al. Bacterial ratchet motors. Proc. Natl. Acad. Sci. USA 107, 9541–9545 (2010).
Chaturvedi, N., Hong, Y. Y., Sen, A. & Velegol, D. Magnetic Enhancement of Phototaxing Catalytic Motors. Langmuir 26, 6308–6313 (2010).
Kummel, F. et al. Circular Motion of Asymmetric SelfPropelling Particles. Phys. Rev. Lett. 110, 198302 (2013).
Wang, W., Duan, W., Ahmed, S., Sen, A. & Mallouk, T. E. From one to many: dynamic assembly and collective behavior of selfpropelled colloidal motors. Acc. Chem. Res. 48, 1938–1946 (2015).
Lauga, E., DiLuzio, W. R., Whitesides, G. M. & Stone, H. A. Swimming in circles: motion of bacteria near solid boundaries. Biophys J. 90, 400–412 (2006).
Drescher, K. et al. Dancing Volvox: Hydrodynamic Bound States of Swimming Algae. Phys. Rev. Lett. 102, 168101 (2009).
Qin, L. D., Banholzer, M. J., Xu, X. Y., Huang, L. & Mirkin, C. A. Rational design and synthesis of catalytically driven nanorotors. J. Am. Chem. Soc. 129, 14870–14872 (2007).
Wang, Y. et al. Dynamic Interactions between Fast Microscale Rotors. J. Am. Chem. Soc. 131, 9926–9927 (2009).
Kummel, F. et al. “Circular Motion of Asymmetric SelfPropelling Particles” Reply. Phys. Rev. Lett. 113, 029802 (2014).
Ebbens, S., Jones, R. A. L., Ryan, A. J., Golestanian, R. & Howse, J. R. Selfassembled autonomous runners and tumblers. Phys. Rev. E 82, 015304 (2010).
Boymelgreen, A., Yossifon, G., Park, S. & Miloh, T. Spinning Janus doublets driven in uniform ac electric fields. Phys. Rev. E 89, 011003 (2014).
Zhang, L. et al. Artificial bacterial flagella: Fabrication and magnetic control. Appl. Phys. Lett. 94, 3079655 (2009).
Pak, O. S., Gao, W., Wang, J. & Lauga, E. Highspeed propulsion of flexible nanowire motors: Theory and experiments. Soft Matter 7, 8169–8181 (2011).
Gao, W., Sattayasamitsathit, S., Manesh, K. M., Weihs, D. & Wang, J. Magnetically Powered Flexible Metal Nanowire Motors. J. Am. Chem. Soc. 132, 14403–14405 (2010).
Gao, W. et al. Bioinspired Helical Microswimmers Based on Vascular Plants. Nano Lett. 14, 305–310 (2014).
Dreyfus, R. et al. Microscopic artificial swimmers. Nature 437, 862–865 (2005).
Soto, R. & Golestanian, R. Selfassembly of active colloidal molecules with dynamic function. Phys. Rev. E 91, 052304 (2015).
Li, F., Josephson, D. P. & Stein, A. Colloidal Assembly: The Road from Particles to Colloidal Molecules andCrystals. Angew. Chem. Int. Edn. 50, 360–388 (2011).
Vutukuri, H. R. et al. Colloidal analogues of charged and uncharged polymer chains with tunable stiffness. Angew. Chem. Int. Edn. 51, 11249–11253 (2012).
Vutukuri, H. R., Imhof, A. & van Blaaderen, A. Fabrication of polyhedral particles from spherical colloids and their selfassembly into rotator phases. Angew. Chem. Int. Edn. 53, 13830–13834 (2014).
Duguet, E., Desert, A., Perro, A. & Ravaine, S. Design and elaboration of colloidal molecules: an overview. Chem. Soc. Rev. 40, 941–960 (2011).
Yethiraj, A. Tunable colloids: control of colloidal phase transitions with tunable interactions. Soft Matter 3, 1099–1115 (2007).
Zerrouki, D., Baudry, J., Pine, D., Chaikin, P. & Bibette, J. Chiral colloidal clusters. Nature 455, 380–382 (2008).
Smallenburg, F., Vutukuri, H. R., Imhof, A., van Blaaderen, A. & Dijkstra, M. Selfassembly of colloidal particles into strings in a homogeneous external electric or magnetic field. J. Phys. Condens. Matter. 24, 464113 (2012).
Peng, B., Vutukuri, H. R., van Blaaderen, A. & Imhof, A. Synthesis of fluorescent monodisperse nonspherical dumbbelllike model colloids. J. Mater. Chem. 22, 21893–21900 (2012).
Biswal, S. L. & Gast, A. P. Mechanics of semiflexible chains formed by poly(ethylene glycol)linked paramagnetic particles. Phys. Rev. E. 68, 021402 (2003).
Byrom, J., Han, P., Savory, M. & Biswal, S. L. Directing Assembly of DNACoated Colloids with Magnetic Fields To Generate Rigid, Semiflexible, and Flexible Chains. Langmuir 30, 9045–9052 (2014).
Gangwal, S., Cayre, O. J. & Velev, O. D. Dielectrophoretic assembly of metallodielectric Janus particles in AC electric fields. Langmuir 24, 13312–13320 (2008).
Ramirez, L. M. et al. Polloidal Chains from SelfAssembly of Flattened Particles. Langmuir 29, 10340–10345 (2013).
Gangwal, S., Cayre, O. J. & Velev, O. D. Dielectrophoretic Assembly of Metallodielectric Janus Particles in AC Electric Fields. Langmuir 24, 13312–13320 (2008).
Hunter, R. J. Foundations of Colloid Science. (Oxford University Press, 2001).
Mazur, S., Beckerbauer, R. & Buckholz, J. Particle size limits for sintering polymer colloids without viscous flow. Langmuir 13, 4287–4294 (1997).
Ebbens, S. et al. Electrokinetic effects in catalytic platinuminsulator Janus swimmers. EplEurophys Lett. 106, 58003 (2014).
Brown, A. & Poon, W. Ionic effects in selfpropelled Ptcoated Janus swimmers. Soft Matter 10, 4016–4027 (2014).
Rogers, S. S., Waigh, T. A., Zhao, X. B. & Lu, J. R. Precise particle tracking against a complicated background: polynomial fitting with Gaussian weight. Phys. Biol 4, 220–227 (2007).
Tirado, M. M., Martínez, C. L. & de la Torre, J. G. Comparison of theories for the translational and rotational diffusion coefficients of rod‐like macromolecules. J. Chem. Phys. 81, 2047–2052 (1984).
van Teeffelen, S. & Lowen, H. Dynamics of a Brownian circle swimmer. Phys. Rev. E 78, 020101 (2008).
Purcell, E. M. Life at low Reynolds number. Am. J. Phys 45, 3–11 (1977).
Goodwin, J., Hearn, J., Ho, C. & Ottewill, R. Studies on the preparation and characterisation of monodisperse polystyrene laticee. Colloid and Polymer Science 252, 464–471 (1974).
Song, J. S., Tronc, F. & Winnik, M. A. Twostage dispersion polymerization toward monodisperse, controlled micrometersized copolymer particles. J. Am. Chem. Soc. 126, 6562–6563 (2004).
Vutukuri, H. R. et al. An experimental and simulation study on the selfassembly of colloidal cubes in external electric fields. Soft Matter 10, 9110–9119 (2014).
Vutukuri, H. R., Badaire, S., Matthijs de Winter, D. A., Imhof, A. & van Blaaderen, A. Directed SelfAssembly of MicronSized Gold Nanoplatelets into Oriented Flexible Stacks with Tunable Interplate Distance. Nano Letters 15(8), 5617–5623 (2015).
Vutukuri, H. R., Stiefelhagen, J., Vissers, T., Imhof, A. & van Blaaderen, A. Bonding assembled colloids without loss of colloidal stability. Adv. Mater. 24, 412–416 (2012).
ten Hagen, B. et al. Can the selfpropulsion of anisotropic microswimmers be described by using forces and torques? J PhysCondens Mat 27, 194110 (2015).
de la Torre, J. G., Huertas, M. L. & Carrasco, B. Calculation of hydrodynamic properties of globular proteins from their atomiclevel structure. Biophysical journal 78, 719–730 (2000).
Bet, B., Boosten, G., Dijkstra, M. & van Roij, R. Efficient shapes for microswimming: From threebody swimmers to helical flagella. J. Chem. Phys. 146, 4976647 (2017).
Rotne, J. & Prager, S. Variational Treatment of Hydrodynamic Interaction in Polymers. J. Chem. Phys. 50, 4831–4837 (1969).
Wajnryb, E., Mizerski, K. A., Zuk, P. J. & Szymczak, P. Generalization of the RotnePragerYamakawa mobility and shear disturbance tensors. J. Fluid Mechanics 731, 402 (2013).
Acknowledgements
We would like to thank Frank Smallenburg for useful discussions. W.T.S.H. acknowledges financial support by the European Research Council Advanced Grant (246812 intercom), H.R.V. was partially supported by a Marie SkłodowskaCurie Intra European Fellowship (G.A. No. 708349 SPCOLPS) within Horizon 2020, and R.v.R. and B.B. by a NWOVICI grant of the Netherlands Organization for Scientific Research.
Author information
Authors and Affiliations
Contributions
H.R.V. conceived the research and designed the experiments. H.R.V. performed all the experiments and analysis. W.T.S.H. supervised the research. B.B., R.v.R., and M.D. developed the numerical models. B.B. performed the calculations. H.R.V., B.B., and W.T.S.H. wrote the manuscript. All authors discussed the results and commented on the manuscript.
Corresponding authors
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Vutukuri, H.R., Bet, B., van Roij, R. et al. Rational design and dynamics of selfpropelled colloidal bead chains: from rotators to flagella. Sci Rep 7, 16758 (2017). https://doi.org/10.1038/s41598017167315
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41598017167315
This article is cited by

Emergent dynamics due to chemohydrodynamic selfinteractions in active polymers
Nature Communications (2024)

Lightswitchable propulsion of active particles with reversible interactions
Nature Communications (2020)

Active particles induce large shape deformations in giant lipid vesicles
Nature (2020)

Direct numerical simulation of the selfpropelled Janus particle: use of gridrefined fluctuating lattice Boltzmann method
Microfluidics and Nanofluidics (2019)

Targeted assembly and synchronization of selfspinning microgears
Nature Physics (2018)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.